**Department of Structures ** **for Engineering and Architecture **

**Department of Structures**

**for Engineering and Architecture**

### P H .D. P ROGRAMME IN

### M ATERIALS E NGINEERING AND S TRUCTURES

### C OORDINATOR P ROF . G IUSEPPE M ENSITIERI

### XXV C YCLE

### C OSTANTINO M ENNA

### P ^{H} .D. T ^{HESIS}

**M** **ULTISCALE ** **D** **AMAGE ** **M** **ODELING OF ** **A** **DVANCED **

**C** **OMPOSITE ** **M** **ATERIALS**

### T

UTORS### : P

ROF### . D

R### . A

NDREA### P

ROTA### P

ROF### . D

R### . C

HARLES### E. B

AKIS### C

O### -T

UTOR### : D

R### . D

OMENICO### A

SPRONE**2013**

*“The process of scientific discovery is, in effect, *
*a continual flight from wonder” *

**Albert Einstein**

**Acknowledgements **

**Acknowledgements**

At the end of this PhD programme, there are many people who deserve gratitude for giving me the possibility to conduct valuable research, acquire new engineering skills, make this work possible and broaden my horizons of knowledge.

Sincere and deep gratitude goes to my advisor Prof. Andrea Prota who, three years ago, motivated me to join the Department of Structures for Engineering and Architecture. I would like to sincerely thank him for giving me guidance during these three years and particularly for his sincere and precious advices to take up fruitful and valuable scientific experiences; without him, I wouldn't have started this “journey”.

Special thanks go also to Prof. Gaetano Manfredi for making this department a very motivating place with exceptional people.

Very special thanks go to Prof. Charles E. Bakis, firstly for the hospitality and the incomparable willingness he has shown me during my visiting research period at the department of Engineering Science and Mechanics of the Pennsylvania State University. His scientific guidance and motivation encouraged me to enthusiastically work on valuable research topics, contributing to increase my love for materials engineering. I am also grateful to Prof. Auricchio, for his precious advices in conducting valuable research activities.

My deepest appreciation goes to my co-tutor, Dr. Domenico Asprone for his invaluable guidance, patience, support and encouragement throughout the course of this research. Through these years Mimmo has become firstly a good friend and a source of precious teachings throughout the wide range of activity conducted during this programme. I really thank him for making things easier than they are!

I would like to also thank all colleagues and roommates at the Department of Structures for Engineering and Architecture who have contributed in many ways to make this period an enjoyable one.

Finally, there is also a “non-academic” part that deserves sincere gratitude for supporting and motivating my choices. Special thanks go to my closer Italian, Canadian and American friends for valuable advices they gave me during these three years. I can never give enough thanks to my parents and my sister whose unconditional love and encouragement never left me during this journey. Lastly, special thanks go particularly to Valeria, for her love, patience on my lack of time on many occasions and especially for the wonderful moments we shared in US during this experience.

**ABSTRACT **

**ABSTRACT**

The use of composite materials has spread over the years throughout the engineering areas of structures. The technological progress in this field has recently expanded, resulting in the design of new composite configurations, including multilayered composite materials and multifunctional nanostructured materials. Even though traditional and emerging composite materials offer wide potentialities for engineering, a significant challenge is still open with respect to damage phenomena.

Driven by safety requirements and cost-effective optimization needs, damage modeling has gained a fundamental role for composite engineering. It represents a strong motivation to support design procedures by means of numerical methods, such as finite element analyses. Recently, multiscale computational analyses effectively gained a major role within the challenging task of damage prediction. Particularly, by bridging physical phenomena occurring at diﬀerent scales, i.e. macro, meso, micro and even nano, damage evolution can be accurately predicted.

The present work is collocated within this scenario with the aim of exploring and
addressing different critical issues related to the failure mechanisms acting at different
length scales of different composite systems. The multiscale procedures, proposed to
evaluate the damage behavior of such materials, involved experimental, analytical and
numerical tools. In detail, damage modeling has been performed for different case
*studies: i) GFRP composite laminates, ii) phenolic impregnated skins/honeycomb *
*Nomex core sandwich structures, iii) Carbon Nanotube/Nanofiber modified S2-*
Glass/epoxy composites.

*For the case study i), the activity concerned the damage occurred in case of low-*
velocity impact tests, carried out on glass fabric/epoxy laminates. In this case, the
multiscale modeling was implemented to account for both intralaminar and
interlaminar levels of damage occurring within the composite laminate. This allowed to
characterize the critical parameters acting at the smaller (interlaminar) scale which

8

hierarchical structure, a multiscale approach was necessary in order to suitably capture damage mechanisms occurring to the composite skins and honeycomb core. The study was firstly aimed at accurately addressing the out-of-plane compressive response;

particularly, in order to evaluate the influence of imperfection variability on the buckling and crushing behavior, a statistics-based approach was proposed and applied to a detailed finite element model of a single representative honeycomb cell.

Furthermore, the impact was also investigated. Finite element numerical models, based on the sandwich assembly structure, were progressively validated through experimental tests, both static and dynamic, performed from the coupon to the sandwich assembly length scale.

*In the case study iii) the multiscale damage modeling procedure was focused on *
some issues related to the Carbon Nanotube/Nanofiber length scale, including
nanotube length and orientation characterization, stress transfer to the matrix and
nanotube toughening mechanisms. A micromechanical model, taking into account
CNT length and orientation distribution, was implemented in order to model mode I
interlaminar fracture toughness of multiscale CNT/CNF S2-Glass/epoxy composites.

For all the investigated case studies the adopted multiscale based strategies revealed to be mostly effective in capturing the most significant damage-related parameters at the lower scales, influencing the structural mechanisms, acting at the structure/component scale.

7CONTENTS ... I LIST OF FIGURES ...IV LIST OF TABLES ...IX

**CHAPTER I... 1 **

**INTRODUCTION ... 1 **

### 1.1. INTRODUCTION ... 1

**1.2. HISTORICAL OVERVIEW AND MULTISCALE DAMAGE ** **ANALYSIS ... 3 **

**1.3. RESEARCH PURPOSES AND OUTLINE ... 6 **

**CHAPTER II ... 11 **

**IMPACT BEHAVIOR OF GFRP COMPOSITE LAMINATES... 11 **

**2.1. INTRODUCTION TO FRAMEWORK ... 11 **

**2.2. LITERATURE OVERVIEW: IMPACT ON COMPOSITE ** **LAMINATES... 12 **

**2.3. IMPACT MODELING ... 15 **

**2.4. MATERIALS AND EXPERIMENTAL METHODS ... 16 **

**2.5. EXPERIMENTAL RESULTS AND DISCUSSION ... 17 **

**2.6. NUMERICAL ANALYSIS ... 22 **

**2.6.1. MODEL FEATURES ... 22 **

**2.6.2. DELAMINATION MODELING ... 25 **

**2.7. ASSESSMENT OF THE MODEL ... 27 **

**2.7.1. CALIBRATION ANALYSIS ... 28 **

**2.7.2. FORCE-DISPLACEMENT CURVES ... 31 **

**2.7.3. DAMAGE ASSESSMENT... 35 **

II

**REFERENCES... 38 **

**CHAPTER III ... 43 **

**OUT OF PLANE COMPRESSIVE BEHAVIOR OF HONEYCOMB **
**SANDWICH STRUCTURES ... 43 **

**3.1. INTRODUCTION TO FRAMEWORK ... 43 **

**3.2. LITERATURE OVERVIEW ... 44 **

**3.2.1. SANDWICH STRUCTURES: INTRODUCTION ... 44 **

**3.2.2. SANDWICH FAILURE MODE: SKIN FAILURE ... 47 **

**3.2.3. SANDWICH FAILURE MODE: CORE FAILURE ... 48 **

**3.2.4. SANDWICH FAILURE MODE: FAILURE MAP ... 49 **

**3.2.5. HONEYCOMB OUT OF PLANE PROPERTIES ... 50 **

**3.2.6. IMPERFECTIONS – CLASSIFICATION AND MODELING ... 55 **

**3.3. MATERIALS AND METHODS ... 59 **

**3.3.1. MODEL FEATURES ... 60 **

**3.3.2. APPROACH VALIDATION ... 64 **

**3.4. RESULT DISCUSSION ... 66 **

**3.4.1. EXPERIMENTAL BEHAVIOR ... 66 **

**3.4.2. NUMERICAL RESULTS: BUCKLING FAILURE MODE ... 69 **

**3.4.3. NUMERICAL RESULTS: CRUSHING ... 84 **

**3.5. CLOSING REMARKS ... 87 **

### REFERENCES... 88

**CHAPTER IV ... 93 **

**IMPACT BEHAVIOR OF HONEYCOMB SANDWICH STRUCTURES**

**93 ** **4.1. INTRODUCTION TO FRAMEWORK ... 93 **

**4.2. LITERATURE OVERVIEW: IMPACT ON SANDWICH ** **STRUCTURES ... 94 **

**4.3. MATERIALS AND METHODS ... 96 **

**4.4. SANDWICH MATERIAL MODELING ... 97 **

**4.4.1. E-GLASS PHENOLIC SKINS ... 98 **

**4.4.2. NOMEX CORE ... 101 **

**4.5. CALIBRATION AND NUMERICAL SIMULATION ... 102 **

**4.5.1. E-GLASS PHENOLIC SKINS – STATIC TESTS ... 103 **

**4.5.2. NOMEX CORE – STATIC TESTS... 107 **

**4.5.3. SANDWICH ASSEMBLY – FOUR POINT BENDING TEST ... 108 **

**4.6. SANDWICH ASSEMBLY – INDENTATION TEST ... 110 **

**4.7. IMPACT ANALYSIS ... 112 **

**4.7.1. DAMAGE ASSESSMENT... 119 **

**4.8. CLOSING REMARKS ... 121 **

**CHAPTER V ... 125 **

**FRACTURE TOUGHNESS OF MULTISCALE CARBON NANOTUBE **
**REINFORCED COMPOSITES ... 125 **

**5.1. INTRODUCTION TO FRAMEWORK ... 125 **

**5.2. CARBON NANOTUBES – BACKGROUND AND INTRODUCTION** **127 ** **5.2.1. CNT LENGTH CHARACTERIZATION ... 128 **

### 5.2.2. CNT

ORIENTATION### ... 137

### 5.2.3. CNT

^{ WAVINESS}

### ... 143

### 5.2.4. CNT-

POLYMER INTERFACIAL SHEAR STRESS### (

LOAD TRANSFER### ) ... 145

### 5.3. ON NANOCOMPOSITE TOUGHNESS ... 148

**5.3.1. CNT FRACTURE TOUGHNESS MODELING ... 154 **

**5.4. CURRENT CNT PULLOUT MODEL... 163 **

### 5.4.1. EXPERIMENTAL VALIDATION ... 171

### 5.4.2. MATERIALS AND EXPERIMENTAL RESULTS [91] ... 172

### 5.4.3. CNT PULLOUT MODEL APPLICATION ... 177

### 5.5. CONCLUDING REMARKS ... 200

**CONCLUSIONS ... 213**

IV

Figure 1.1: Multiscale procedure for the design and optimization of multilayered composite
structures: a) increasing the scale levels of the composite component; b) type of tests and
analyses to be performed as the length scale increases. ... 5
*Figure 1.2: Concept of multiscale strategies applied to nanostructures: a) [7]; multiscale *

simulation strategy for coarse-graining of surfactant molecules into beads b) [8]... 6 Figure 2.3: Scheme of multiscale damage analysis for GFRP laminates adopted within the

study. ... 12 Figure 2.4: Typical impact damage in a composite laminate: a) failure due to fiber breakage [4];

b) intralaminar matrix shear cracks [5]; c) delaminations between adjacent plies [4]. ... 14 Figure 2.5: Illustration of impact damage development: a) damaged area through the thickness

of the composite laminate; matrix cracks (red) and delamination (blue) pattern for
transverse impact b), c) [6]. ... 15
*Figure 2.6: Schematic representation of the GFRP stacking sequence with n=1, a) and n=2, b).*

... 17
*Figure 2.7: Effect of the laminate thickness, t, on the F-d curves. ... 18*
*Figure 2.8: Effect of the energy level, U, on the F-d curves. Laminate thickness t=0.96mm. ... 19*
*Figure 2.9: Absorbed energy, U**d**, vs impact energy, U. ... 19*
Figure 2.10: Visible damaged area of an impacted panel. ... 20
*Figure 2.11: Extent of ply-by-ply delaminated area, A**m**. Panel thickness t=1.92mm; impact *

*energy U=20.0 J. ... 21*
*Figure 2.12: Characteristic dimension of projected delaminated area, d, vs impact energy, U. . 21*
*Figure 2.13: Projected delaminated area, A**p**, vs impact energy, U. ... 22*
Figure 2.14: Stress profile a) and damage evolution law b) of TieBreak contact [31]. ... 26
Figure 2.15: FE model set up adopted in the numerical analysis. ... 27
*Figure 2.16: Comparison of experimental and numerical F-d curves for the 0.96 mm thick *

*laminate; a) U=0.4J; b) U=1.5J; c) U=3.3J; d) U=4.0J; e) U=6.0J. ... 31*
*Figure 2.17: Comparison of experimental and numerical F-d curves for the 1.92 mm thick *

*laminate; a) U=0.8J; b) U=8.3J; c) U=12.4J; d) U=15.5J; e) U=20.0J. ... 34*
Figure 2.18: Comparison of: a) experimental, and, b) calculated delaminated area. Laminate

thickness t=0.96 mm; impact energy U=6.0 J. ... 36
*Figure 2.19: Interlaminar damage of the 1.92 mm thick laminate impacted at U=15.5J: a) *

through the thickness shear failure; b) exploded laminate view depicting longitudinal
*tensile failure, X direction; c) bottom view of composite laminate, longitudinal tensile *
*failure, X direction; d) post impact view. ... 37*
Figure 3.20: Scheme of multiscale analysis performed for the investigated Nomex honeycomb

structure. ... 44

Figure 3.21: Schematic representation of a sandwich structure ... 45 Figure 3.22: Skin failure modes: a) compressive failure; b) intra-cell buckling; c) wrinkling

failure [20]. ... 48
Figure 3.23: Core failure modes: a) shear failure; b) indentation failure [20]. ... 49
*Figure 3.24: Schematization of the plastic buckling of a honeycomb loaded in Z(3) direction a); *

work dissipated in the plastic hinge b). ... 54
Figure 3.25: Expansion manufacturing process for honeycomb material [7]. ... 55
Figure 3.26: Corrugated manufacturing process for honeycomb material [7]. ... 56
*Figure 3.27: a) in plane periodical honeycomb microstructure for hexagonal cells, W-L plane; b) *

single representative periodic cell; c) 3D finite element mesh rendering for a single Nomex honeycomb cell. ... 61 Figure 3.28: SEM photos of Nomex™ core. a) Transverse section; b) detail of a vertex of a

hexagonal cell [40]. ... 63
Figure 3.29: Schematic flow chart of the simulation strategy. ... 65
Figure 3.30: a) compressive stress – strain, * _{c}* vs /h, response for HRH 10-1/8-3.0 hexagonal

Nomex honeycomb; b) sequence of photographs of honeycomb cells at different stages of
axial compressive strain. ... 68
Figure 3.31: a) compressive stress – strain, * _{c}* vs /h, response for Hexcel Al-5052-H39

hexagonal aluminum honeycomb; b) focus on critical buckling load; c) focus on
compressive strength; d) first (A), second (B) buckling mode and plasticized cell (C) as a
result of the current approach. ... 71
Figure 3.32: compressive stress – strain, *c* vs /h, response for HRH 10-1/8-3.0 hexagonal

Nomex honeycomb up to folding with FE results of cell deformations corresponding to
A=critical buckling limit, B=shape up to compressive strength, C1-C5=strain localization
for the five cell samples, D=first fold of the cell. ... 72
Figure 3.33: Effect of thickness variability on * _{c}* vs /h curves for a) CV=10%, b) CV=15%, c)

CV=20%, d) CV=25% with the corresponding PDF and focusing on the peak of
compressive strength; e) superposition of CV=10% and CV=25% cases. ... 76
Figure 3.34: Effect of Young’s modulus variability on *c* vs /h curves for a) CV=10%, b)

CV=15%, c) CV=20%, d) CV=25% with the corresponding PDF and focusing on the peak
of compressive strength; e) superposition of CV=10% and CV=25% cases. ... 79
Figure 3.35: Effect of both thickness and Young’s modulus variability on * _{c}* vs /h curves for a)

CV=10%, b) CV=15%, c) CV=20%, d) CV=25% with the corresponding PDF and focusing on the peak of compressive strength; e) superposition of CV=10% and CV=25%

cases. ... 82 Figure 3.36: a) average computed compressive strength vs CV adopted for Nomex properties;

b) average computed Young’s modulus vs CV adopted for Nomex properties; c) CV on computed compressive strength vs CV adopted for Nomex properties. ... 84 Figure 3.37: Full Stress-Strain relationship for Nomex honeycomb material – experimental

VI

contact between walls (point 3), c) double contact between walls (point 5), d) final deformed shape. ... 87 Figure 4.39: Scheme of multiscale damage analysis conducted on Honeycomb sandwich

structure. ... 94 Figure 4.40: Shape geometry of hexagonal honeycomb core. ... 97 Figure 4.41: a) Stress vs Strain relationship for single element tensile test (direction 1) for

*different values of E**1**T, b) correspondent damage variable ω**1* vs strain relationship. ... 101
Figure 4.42: Stress vs Strain relationship for tensile a) warp, b) weft, c) in plane shear direction

*and corresponding damage variable, ω, evolution ranging from 0 (blue) to 1 (red). ... 106*
Figure 4.43: Compressive Stress vs Strain curve for the Nomex core. ... 107
Figure 4.44: Load vs Deflection curve for the four point bending test. ... 109
*Figure 4.45: Contour of a) LT stress in the Nomex core, b) L direction stress in the upper and *

lower skin. ... 110 Figure 4.46: Load vs Deflection numerical and experimental curve for the static indentation test

a); through the thickness stress distribution before b) and after c) Nomex crushing. ... 111
*Figure 4.47: a) Comparison of experimental and numerical F-d curves for t=1 mm, d=12.7 mm, *

*v=4 m/s with numbered sequence of sandwich damage mechanisms; b) corresponding *
energy displacement curve. ... 114
Figure 4.48: Fringe level of strain rate in warp direction a) and distribution of effective strain

*rate on the upper skin (t=1 mm, d=12.7 mm, v=4 m/s). ... 115*
*Figure 4.49: Simulated damage sequence occurring in the E-glass phenolic sandwich with t=1 *

*mm, d=12.7 mm, v=4 m/s (contour of plastic strain): 1) Nomex crushing, 2) Top skin *
failure, 3) Shear failure in the Nomex core, 4) Plug formation, 5) Bottom skin failure, 5)
Complete penetration. ... 116
*Figure 4.50: Comparison of experimental and numerical F-d curves for t=1mm, d=12.7mm, *

*v=8m/s with evolution of damage variable ω**1** and ω**12.* ... 118
*Figure 4.51: Comparison of experimental and numerical F-d curves for a) t=2 mm, d=12.7 mm, *

*v=1 m/s and b) t=2 mm, d=12.7 mm, v=4 m/s. ... 118*
*Figure 4.52: Comparison of experimental and numerical F-d curves for t=1 mm, d=20.0 mm, *

*v=8 m/s and corresponding top view of impacted specimens. ... 119*
Figure 4.53: Comparison of experimental a) and numerical b) top residual damage for E-glass

*phenolic sandwich with t=1 mm, d=12.7 mm, v=8 m/s. ... 120*
Figure 4.54: Comparison of experimental a) and numerical b), through the thickness residual

*damage for E-glass phenolic sandwich with t=2mm, d=12.7mm, v=1m/s. ... 120*
Figure 5.55: Illustration of multiscale framework of damage analysis for Mode I interlaminar

fracture toughness of CNT/CNF-based composites. ... 126 Figure 5.56: Schematic representation of the SWCNT and MWCNT structure: a) definition of

chiral vectors and chiral angle [5], b) three dimensional rendering. ... 128

Figure 5.57: a) AFM analysis of dispersions of CNTs in 0.5% SDBS, b) simultaneous length and diameter measurements [23]. ... 132 Figure 5.58: Comparison of length distributions before (pristine MWCNTs) and after

processing of NanocylTM NC7000 a) and Baytube b) C150HP MWCNTs [31]. ... 133 Figure 5.59: PDF for different scale and shape parameters: Lognormal a) and Weibull

distribution b). ... 136 Figure 5.60: Histogram of dispersed SWNT lengths [34]. ... 137 Figure 5.61: Definition of Euler angles in SWNT nanocomposites [36]. ... 138 Figure 5.62: Incident and scattered intensities on the SWNT and related angles in the polymer

and laboratory frames [36]. ... 141 Figure 5.63: The spring model of a curved CNT [56]. ... 144 Figure 5.64: RVE for wavy CNT embedded in polymer matrix [59]. ... 145 Figure 5.65: Detail of an MD model: a) cross-sectional view of the model, b) CNT pull-out

from polymer matrix [74]. ... 147 Figure 5.66: Schematic description of possible fracture mechanisms of CNTs [80]: (a) initial

state of the CNT; (b) CNT pull-out due to CNT/matrix; (c) rupture of CNT ; (d) sword in sheath mechanism, i.e. fracture of the outer CNT layer and pull-out of the inner tube; (e) bridging and partial debonding of the interface. ... 150 Figure 5.67: TEM micrographs of MWCNTs bridging a matrix crack; the inset highlights

MWCNT pullout from the matrix [81]. ... 150 Figure 5.68: Schematic representation of a crack propagating in a composite: through a micro- fiber a) and a certain number of CNTs b) having total volume equivalent to the volume of the microfiber. ... 152 Figure 5.69: Schematic illustration of a single fiber pullout. ... 152 Figure 5.70: Relationship between the pull-out force and pull-out displacement for a MWCNT

being pulled out from its surrounding matrix [85]. ... 156 Figure 5.71: Pull-out force and displacement curve MWCNT sword in sheath mechanism [85].

... 156 Figure 5.72: Linear bridging law for pullout of CNTs [86].: ... 157 Figure 5.73: Mathematical illustration of equations 5.21 and 5.22 (MWCNT pullout and sword

in sheath mechanism) [86]. ... 158 Figure 5.74: Schematic representation of CNF/CNT filled epoxy resin interlayer placed at the

midplane of the composite laminate (highlighted in red); a) S2-glass fiber/epoxy laminated composite, b) focus on the nanofilled epoxy interlayer placed at the midplane of the laminate. ... 163 Figure 5.75: Illustration of the CNT-bridged Mode I IFT specimen, a); focus on the CNF/CNT

bridging action during crack propagation, b). ... 165 Figure 5.76: Scheme of CNT pullout problem: a) pullout of different CNTs within the resin

VIII

*direction, P. ... 167*
Figure 5.77: PDF for CNT orientation distribution: equation 5.31 reported for different scale

and shape parameters. ... 168
*Figure 5.78: Increment of the onset of damage G**Io* for the mode I IFT test ... 175
Figure 5.79: SEM images of mode I fracture surfaces [91]: a) composite with a long GPS-CNT

epoxy interlayer; b) long GPS-CNTs in the interlayer: cavities in circles were possibly created by CNT pull-out; c) composite with a GPS-CNF interlayer; d) GPS-CNFs with epoxy layers bonded to the CNF surface. ... 177 Figure 5.80: CNF details: a) 3D rendering; b) longitudinal section; c) TEM image and material

characteristics - (from *Applied * *Sciences * *Inc. * *(Cedarville, * *OH) *
http://apsci.com/?page_id=19). ... 178
Figure 5.81: UF-CNF length distribution after 1 and 4 hours of bath sonication dispersion time

according to the length distribution of equation 5.28. ... 179
*Figure 5.82: Short OH Functionalized material properties and Short OH TEM image; provided *

*by http://www.cheaptubesinc.com/shortohcnts.htm#ixzz2HkbOislo ... 180*
*Figure 5.83: VGCNTs material properties and VGCNTs TEM image; provided by *

http://www.cheaptubesinc.com/shortohcnts.htm#ixzz2HkbOislo ... 180 Figure 5.84: Probability density distribution of a-MWCNTs (i.e. VGCNTs) after 5 minutes of

sonication in epoxide/acetone mixture [96]. ... 181
*Figure 5.85: Increment of fracture energy (G**Ionset* increment) as a function of interfacial shear

strength : Case 1 (baseline material properties, Table 5.11)... 185
*Figure 5.86: Increment of fracture energy (G**Ionset* increment) as a function of interfacial shear

strength *: Case 1 (variation of V**CNF*)... 186
*Figure 5.87: Increment of fracture energy (G**Ionset* increment) as a function of interfacial shear

strength *: Case 1 (variation of L**C*). ... 187
*Figure 5.88: Increment of fracture energy (G**Ionset* increment) as a function of interfacial shear

strength *: case 1 (variation of d**CNT*). ... 188
*Figure 5.89: Increment of fracture energy (G**Ionset* increment) as a function of interfacial shear

strength : case 1 (variation of *CNT*). ... 188
*Figure 5.90: Increment of fracture energy (G**Ionset* increment) as a function of interfacial shear

strength : case 1-2, comparison of Fu and Lauke model and Mirjalili model by assuming
modified input material data. ... 191
*Figure 5.91: Increment of fracture energy (G**Ionset* increment) as a function of interfacial shear

strength : Case 4 (baseline material properties, Table 5.12)... 193
*Figure 5.92: Increment of fracture energy (G**Ionset* increment) as a function of interfacial shear

strength *: Case 4 (variation of V**CNF*)... 193
*Figure 5.93: Increment of fracture energy (G**Ionset* increment) as a function of interfacial shear

strength *: Case 4 (variation of L**C*). ... 194

*Figure 5.94: Increment of fracture energy (G**Ionset* increment) as a function of interfacial shear

strength *: Case 4 (variation of d**CNT*). ... 195

*Figure 5.95: Increment of fracture energy (G**Ionset* increment) as a function of interfacial shear
strength : Case 4 (variation of * _{CNT}*). ... 195

*Figure 5.96: Increment of fracture energy (G**Ionset* increment) as a function of interfacial shear
strength : Case 4, comparison of the Fu and Lauke model and the Mirjalili model by
assuming modified input material data. ... 197

*Figure 5.97: Increment of fracture energy (G**Ionset* increment) as a function of interfacial shear
strength : Case 3, comparison of Fu and Lauke model and Mirjalili model by assuming
modified input material data. ... 199

*Figure 5.98: Increment of fracture energy G**Ionset* as a function of average CNT length, L*average*:
Case 3, comparison of the Fu and Lauke model varying interfacial shear strength,
values. ... 200

Figure 5.99: a) MD initial system for CNT pullout at an angle from an epoxy matrixb) three dimensional rendering. ... 202

**List of tables **

Table 2.1: Mechanical properties of the calibrated model. ... 28
**List of tables**

Table 3.2: Failure equation for three-point bending configuration [20]. ... 50

Table 3.3: Mechanical properties of Nomex Honeycomb – experimental results. ... 67

Table 4.4: Test methods involved in the mechanical characterization of skin materials. ... 104

Table 4.5: Mechanical properties of composite skins derived by experimental tests and calibrated parameters (in parenthesis) ... 104

Table 5.6: Comparison of toughness mechanisms of micro- and nano-reinforced polymer matrix composites [79]. ... 149

Table 5.7: Functionalized nanofillers used for making multi-scale reinforced composites ... 173

Table 5.8: Multiscale nanofiler-composite composition and sonication time ... 173

Table 5.9: Mode I IFT test results ... 175

Table 5.10: Mechanical properties of CNTs used within the present study... 181

Table 5.11: Input material data for case 1, 0.5 wt% UF-CNF epoxy, baseline material properties. ... 184

Table 5.12: Input material data for case 4, 0.25 wt% long GPS-CNTs epoxy, baseline material properties. ... 192 Table 5.13: Input material data for case 3, 0.5 wt% short GPS-CNTs epoxy, baseline material

X

**Chapter I **

**Chapter I**

**INTRODUCTION **

**INTRODUCTION**

**1.1. ** **Introduction **

Composite systems, such as fiber reinforced polymers, have increasingly advanced since early developments in the 1970s up to date, gaining the leadership in the lightweight structure engineering field. The aeronautics industry is certainly one of the major recipients of engineering and technological progresses of composite materials; in fact, today, aircrafts such as Boeing 787 and Airbus A380 represent the demonstration of such developments. The use of composite materials has over the years expanded beyond the aerospace applications to other areas of structures. Typical and emerging applications of composite materials include automotive, naval and wind energy sectors, whose future challenges are related to cost effectiveness, multiaxial fatigue resistance, long term durability and structural safety.

The concept of composite systems has expanded over the years resulting in the design of new composite configurations. For instance, the demand for light-weight efficient and high-stiffness structures led to the introduction of multilayered composite configuration, such as sandwich structures. Sandwich structures experienced a wide expansion over the years, still active up to date, especially for applications requiring high stiffness-to-weight ratios; the exclusive properties of core materials, such as honeycomb and foam materials, as well as the high mechanical properties of fiber reinforced composite facesheets, can be suitably tailored and combined to produce cost-effective lightweight components of complex geometries, offering varied physical

2

and mechanical performances (e.g. energy absorption and stiffness optimization, thermal insulation, acoustic damping).

In early 1990s, the development of nanotechnologies pushed research and
engineering community to investigate the high potentialities of multifunctional
*nanostructured materials. In this way, the concept of “composite” material experienced *
a further evolution, with the possibility to incorporate nanofillers (e.g. carbon
nanotubes, nanoparticles, nanoclay) to conventional composite systems, broadening the
typical engineering applications of composites. However, the main concern related to
these promisingly applications is associated with the small dimensional scale of the
filler (the order of magnitude is between 5 and hundreds nm) that need great attention
in order to have fully control of such type of innovative materials.

Even though positive aspects related to the use of composite materials offer wide perspectives for engineering, a significant challenge is still open with respect to damage phenomena; these represent a source of complexity due to significant heterogeneities and interactions between composite constituents. In fact, it is well known that the characterization of failure behavior of composite structures depends on a very large number of variables. For instance, the possibility of having interacting failure modes in a composite laminate constraints the damage analysis to properly characterize intralaminar and interlaminar damage, in order to assess the composite damage behavior. Moreover, with regard to the behavior of sandwich structures, the specific morphology of a sandwich configuration shall be taken into account. The assessment of the global behavior and local stress fields of sandwich structures depends on the material properties of the constituents (skins, core, and adhesive if involved), geometric dimensions, and type of loading. On the contrary, an exhaustive comprehension of damage mechanisms occurring at nanoscale, is the key step for the future effective development and control of nanocomposites systems.

In the light of these considerations, it appears that the modeling of damage and fracture plays an important role for composite engineering development affecting both design stages (to prevent in service damage) and the implementation of structural health monitoring systems (to predict the residual lifetime of structures). Therefore, the main challenge in any computational design procedure is to accurately incorporate damage and its effects on composite structure. In this context, the progress consists in taking advantages of properly modeling damage into computational design procedures with the final aim to reduce the cost of certification requirements and design safer and cost effective structures.

**1.2. Historical overview and multiscale damage analysis **

The mechanisms of damage taking place in a composite system and their effects on mechanical response represent the main challenging concern in the field of composite damage analysis and modeling. These issues developed starting in the 1980s. Before 1980s, the composite failure analysis was mostly based on the continuum mechanics approach extended by previous theories valid for metals. In the 1980s the need to consider the heterogeneous nature of composite materials led to the introduction of micromechanics and continuum damage mechanics theories which were firstly applied to multiple cracking observed in composite materials. The first pioneering work in this field was provided by Aveston et al. [1] who evaluated the role of composite constituent properties, i.e. fibers and matrix properties, relative volume fractions and fiber diameter in resisting multiple cracks in steel fibers reinforced cement composites.

From these concepts, two main advancements were subsequently presented in the approach, namely micro damage mechanics [2] (investigating local ply stress fields to evaluate the overall stiffness degradation) and macro damage mechanics [3]

(investigating internal material discontinuities through the definition of a damage scalar variable). Homogenization techniques were then applied to composite materials [4]; according to this approach, the reinforcement in a composite is treated as a part of the microstructure and is homogenized in a representative volume element as an anisotropic medium in which damage entities are considered. Many further developments have taken place up to the current knowledge in composite material damage field. Clearly, complex structural geometries, composite configurations and load conditions require numerical structural analysis. However the analysis of composite damage behavior, obtained by means of numerical approaches, is rather difficult due to the intrinsic complexity of the interaction of failure modes, damage development and multilayered configurations.

Recently, the advancements achieved in the field of numerical methodologies as
*well as computational efficiency, have motivated the rise of the so called “multiscale” *

computational analysis. The key concept is that physical phenomena occurring at lower length scale control the material response at higher length scales. The heterogeneous nature of composite systems makes multiscale modeling methodologies optimal candidates for these materials. By formulating models at diﬀerent scales, i.e. macro, meso, micro and even nano, damage evolution can be accurately predicted. A wide literature on multiscale modeling exists providing a wide range of results which point

4

descriptions of the behavior of many complex systems [5-7].

In industrial sectors, such as the aerospace industry, the issue of structural
modeling, including static strength prediction, durability analysis and damage tolerance
of composite and sandwich materials, is often addressed through a multiscale method
*based on a complex mix of testing and analysis. This process is also named building *
*block approach or virtual testing which develops according to the flow chart reported *
in Figure 1.1a,b. Tests and numerical analyses are performed progressively at various
levels of structural complexity, starting from small material coupons and moving
through structural elements, sub-components, components, and, finally, up to the
complete full-scale product. Each level uses the experimental/numerical outcomes
gained at the previous level of analysis in order to generate composite material
properties and appropriate analysis methods. For instance, in case of sandwich
structures, the first level of analysis has the objective to characterize of basic material
properties (including skins and core materials) to be used as input data at the assembly
level of analysis. Then, tests and analyses performed at the element level are used to
investigate and validate of both analytical and numerical predictions, with particular
emphasis on the failure modes; at the sub-component level, tests and failure analysis
are implemented to deal with specific geometrical, loading, and environmental
conditions (e.g. fatigue, impact loading, hygrothermal aging). Finally, at the highest
level of structural complexity, tests are used to validate the analysis methods developed
during the previous levels. As the structural complexity rises up, testing costs increase
as well, but the number of tests decreases and more reliable numerical simulations are
validated.

Recently, other features of multiscale approach have emerged in case nanocomposite systems. Nanofillers, thanks to their exceptional properties, offer the possibility to achieve outstanding improvements if added to polymer matrices at much lower concentrations than traditional (micro-sized) fillers. The resulting physical and chemical properties of nanocomposites can be related to the hierarchical structure of this kind of materials. Moreover, nanomodified polymers can be used for the development of nano-modified composite laminates achieving higher performance materials. The engineering progress in the field of nanocomposites requires models capable of accounting for their multiscale structure ranging from the nano to the macro length scales.

*a) *

*b) *

**Figure 1.1: Multiscale procedure for the design and optimization of multilayered **
**composite structures: a) increasing the scale levels of the composite component; b) type of **
**tests and analyses to be performed as the length scale increases. **

In this way, characteristic phenomena acting at each length-scale could be taken into account and their effects bridged from the smaller scale to the macroscale. By accounting for these features, an effective modeling can be achieved. Quaresimin et al.

[7] proposed a classification of the multiscale modeling strategies in the field of nanocomposites, as reported in Figure 1.2:

*- Micromechanical modeling strategies, based on micromechanical models only. *

The matrix and the nanofiller are described by means of continuum mechanics without accounting for interfacial interactions and nanostructure.

6

*- Nanostructural modeling strategies, making use of both micromechanical *
models and nanostructural models. These methods account for the effects of
the inherent nanostructure on the overall macroscopic properties, but
chemical–physical interactions are not taken into account.

*- Molecular modeling strategies, making a combined use of all the above *
mentioned models. Intermolecular and supramolecular interactions are
accounted for by means of discrete methodologies at the actual nanoscale
level.

*a) * *b) *

**Figure 1.2: Concept of multiscale strategies applied to nanostructures: a) [7]; multiscale ****simulation strategy for coarse-graining of surfactant molecules into beads b) [8]. **

**1.3. Research purposes and outline **

In the present work, different critical issues, related to damage assessment and modeling of advanced composite structures, are addressed through the analysis of different case studies in a multiscale procedure. Hereafter, an outline including each case study is presented.

* The activity presented in Chapter II is aimed at simulating the response of *
clamped circular GFRP plates of two different thickness values, struck at low-velocity
by a rigid hemispherical projectile. The design of advanced composite structures or
components subjected to impact loadings requires a deep understanding of the damage
and degradation mechanisms occurring within the composite material. The multiscale

*numerical analysis proposed in Chapter II is aimed at properly including the possible *
modes of failure of the GFRP composite laminates and quantify the energy dissipated
by different mechanisms. Through the definition of suitable finite element models for
both composite plies and interlaminar connections two levels of composite damage
analysis are taken into account:

*- intralaminar level, related to the damage occurring to the matrix and fibers *
within a composite ply;

*- interlaminar level, related to the damage occurring within the matrix layer *
between two adjacent plies.

This numerical approach allows to characterize the critical parameters acting at the smaller (interlaminar) scale, which affect the whole impact response of the composite laminate, at the larger scale. In this way, the energy absorbed by the composite laminate during impact (that is measurable at the larger scale) is related to damage mechanisms occurring within the laminate (that are analyzed at the smaller scale).

* The activities presented in Chapter II and Chapter III have the objective to *
model the mechanical behavior of E-glass phenolic skins/Nomex honeycomb core
sandwich structures, particularly focusing on out of plane compressive properties
(including buckling and crushing) and impact behavior. In detail, the damage analysis

*honeycomb structures; the multiscale numerical analysis moves from the meso scale level, focusing on Nomex paper material properties, including the sensitivity to material defects. Then, the numerical analyses are performed on a representative honeycomb cell enabling to transfer mechanical properties, predicted at the meso scale, to the macroscale of the whole sandwich structure, with the final aim of predicting the compressive strength and folding mechanism during the Nomex cell crushing. The key aspect proposed in the study is the inclusion of imperfections in terms of both material (elastic modulus variability) and geometrical (thickness variability) defects through a stochastic approach: random sampling at each element of the FE mesh are performed assuming different Young’s modulus values and different thickness properties, according to a pre-defined statistical distribution. The modeled cell is used to address several aspects of the compressive response, particularly focusing on the onset of buckling, the collapse limit and the crushing behavior.*

**conducted in Chapter III focuses on the buckling and crushing behavior of hexagonal*** The damage analysis conducted in Chapter IV moves to the scale length of the *
sandwich assembly aimed at modeling the impact behavior of Nomex honeycomb core
combined with E-glass phenolic facesheets. Since the impact damage occurring in

8

approach involves the detailed (static and dynamic) modeling of both skin and core material properties. The adopted multiscale virtual testing procedure is based on the progressive validation of the composite facesheet and orthotropic honeycomb material models on the basis of experimental tests, ranging from coupon tests (for E-glass phenolic skins and Nomex core) to sandwich assembly tests. This allows to verify the capability of the model to take into account the main damage mechanisms taking place during impact. The dynamic impact behavior is then validated through different impact conditions; some important issues on the strain rate sensitiveness affecting the investigated materials are addressed, along with the assessment of energy absorption and damage mechanisms.

* Chapter V investigates the main issues related to the multiscale modeling of *
nanocomposite properties. In detail, the activity focuses on multiscale modeling of
Mode I interlaminar fracture toughness of S2-glass fiber/epoxy laminated composite
modified using nanofillers (Carbon NanoTubes, CNTs, and Carbon NanoFibers,
CNFs) with/without surface functional groups and with different ranges of aspect ratio.

The smaller scale of the analysis takes into account the toughening mechanisms acting at the nanoscale. A suitable analytical model describing the CNT pullout mechanism is then presented accounting for the CNTs properties within the matrix at the nanoscale, i.e. length and orientation distribution and stress transfer.Then, the result of this modeling is used to calibrate fracture energy models at the macroscale, by means of Mode I interlaminar fracture toughness tests on nanofilled S2- glass fiber/epoxy laminated composites. Some important issues are discussed, including interfacial shear stress determination, CNT/CNT volume fraction as well as CNT critical length definition.

**References **

1. *Aveston, J., G.A. Cooper, and A. Kelly, Single and multiple fracture. In: The *
Properties of Fiber Composites (Surrey, UK: IPC Science and Technology
Press, National Physical Laboratory), 1971: p. 15-26.

2. *Hashin, Z., Analysis of cracked laminates: a varational approach. Mechanics *
**of Materials, 1985. 4(2): p. 121-136. **

3. *Kachanov, L.M., Rupture time under creep conditions. Izv Akad Nauk SSSR *
**Otd Tekhn Nauk [in Russian], 1958. 8: p. 26-31. **

4. *Talreja, R., Transverse cracking and stiffness reduction in composite *
**laminates. Journal of Composite Materials, 1985. 19: p. 355-375. **

5. *Zinno, A., E. Fusco, A. Prota, and G. Manfredi, Multiscale approach for the *
*design of composite sandwich structures for train application. Composite *
**Structures, 2010. 92(9): p. 2208-2219. **

6. *Feraboli, P., F. Deleo, et al., Predictive modeling of an energy-absorbing *
*sandwich structural concept using the building block approach. Composites *
**Part a-Applied Science and Manufacturing, 2010. 41(6): p. 774-786. **

7. *Quaresimin, M., M. Salviato, and M. Zappalorto, Strategies for the assessment *
*of nanocomposite mechanical properties. Composites Part B-Engineering, *
**2012. 43(5 ): p. 2290-2297. **

8. *Fermeglia, M. and S. Pricl, Multiscale molecular modeling in nanostructured *
*material design and process system engineering. Computers & Chemical *
**Engineering, 2009. 33(10): p. 1701-1710. **

10

**Chapter II **

**Chapter II**

**IMPACT BEHAVIOR OF GFRP COMPOSITE ** **LAMINATES **

**IMPACT BEHAVIOR OF GFRP COMPOSITE**

**LAMINATES**

**2.1. Introduction to framework **

The design of advanced composite structures or components subjected to impact loadings requires a deep understanding of the damage and degradation mechanisms occurring within the composite material. Despite years of extensive research around the world, a complete and validated methodology for predicting the behavior of composite structures, including the effects of damage, has not yet been fully achieved.

This is largely due to the complexity of the physical phenomena involved, requiring an effective modeling of dynamic effects, material-projectile contact, failure modes development and interaction within the laminate, yet taking into account the influence of impactor geometry, velocity, and mass, and target geometry, constraint conditions, and lay-up.

Damage in a composite laminate generally involves two levels of analysis:

*- intralaminar level, related to the damage occurring to the matrix and fibers *
within a composite ply;

*- interlaminar level, related to the damage occurring within the matrix layer *
between two adjacent plies.

This peculiarity makes suitable a multiscale approach aimed at properly including the
possible modes of failure of the laminate and quantifying the energy dissipated by the
*different mechanisms. The multiscale modeling approach presented in Chapter II is *
conducted including both levels of damage analysis through the definition of suitable

12

finite element models for the composite plies and interlaminar connections, as depicted in Figure 2.3.

**Figure 2.3: Scheme of multiscale damage analysis for GFRP laminates adopted within the **
**study.**

By using this approach, the composite impact behavior is studied at two scales.

This allows to characterize the critical parameters acting at the smaller (interlaminar) scale and affecting the whole impact response of the composite laminate at the larger scale. The energy absorbed by the composite laminate during impact (that is measurable at the larger scale) is related to damage mechanisms occurring within the laminate (that are analyzed at the smaller scale).

In details, the present activity is aimed at simulating the response of clamped circular GFRP plates of two different thickness values, struck at low-velocity by a rigid hemispherical projectile. A finite element model, based on the commercial tool LS- DYNA, is built and calibrated using the information gathered from a minimum of experimental data. Solid finite elements combined with orthotropic failure criteria are used to model the composite failure and stress based contact failure between plies are adopted to model the delamination mechanism.

**2.2. Literature overview: impact on composite laminates **

The use of fiber-reinforced composite materials has increased over the last decades, due to their advantageous specific mechanical properties and corrosion resistance. Advanced composites have been used in many different engineering applications encompassing military, automotive and naval industry, and especially in aerospace, where weight reduction is one of the most important design parameters.

Although these materials offer very attractive properties, their application is often restricted by their vulnerability to transverse impact [1], forcing the adoption of large safety factors and resulting in significantly over-designed structures.

Aeronautical components are prone during service to foreign object impact events [1], varying in the range of low to high velocities and impacting masses, consisting of dropping tools during production, repair or maintenance operations, ice particles or runway debris, bird strikes. At high velocity, the structural response is dominated by the stress wave propagation through the thickness of the laminate, and the resultant damage is quite localized. On the contrary, in a low-velocity impact the contact duration is long enough to excite the global structural response, leading to a more diffuse damage [2, 3].

The damage suffered by a composite laminate subjected to impact loading can affect the composite material within each lamina of the laminate, i.e. intralaminar damage, or it can develop between adjacent plies, i.e. interlaminar damage. Within this distinction, the damage can be divided into four distinct groups:

* matrix cracking, where cracking occurs parallel to the fibers due to tension, *
compression or shear;

* delamination between adjacent plies which is produced by interlaminar *
stresses;

* fiber breakage due to tension fiber breakage and compression fiber buckling; *

* perforation, where the impactor completely perforates the impacted surface. *

Such order corresponds to the damage sequence occurring for increasing impact energies. Figure 2.4 reports SEM images depicting the typical damage occurring in a composite laminate as a consequence of impact, referring to fiber breakage (a), matrix cracking (b) and delamination (c), respectively.

14
*c) *

**Figure 2.4: Typical impact damage in a composite laminate: a) failure due to fiber **
**breakage [4]; b) intralaminar matrix shear cracks [5]; c) delaminations between adjacent **
**plies [4]. **

If the impact energy increases, the damage pattern develops as truncated conical shape with wider damage taking place at the bottom of the panel (Figure 2.5a).

Matrix damage is the first type of failure that occurs during transverse low-velocity impact; it typically takes the form of matrix cracking but also debonding between fiber and matrix within the lamina. Matrix cracks take place due to property mismatching between the fiber and matrix, and are usually oriented in planes parallel to the fiber direction in unidirectional layers. Joshi and Sun [6] provided a typical shear (red), flexural (green) matrix crack and delamination pattern (blue), as shown in Figure 2.5b and c.

*a)*

Impact damage envelope Damage growth (fatigue)

IMPACT

Composite layer directions

*b) * *c)*

**Figure 2.5: Illustration of impact damage development: a) damaged area through the **
**thickness of the composite laminate; matrix cracks (red) and delamination (blue) pattern **
**for transverse impact b), c) [6].**

Delamination, occurring at moderately low energy levels, deserves serious considerations, being able to cause a significant decrease in the static material compression strength, or growing under cyclic loads leading to a gradual loss in strength and stiffness [7].

**2.3. Impact modeling **

The impact response of composite laminates has been widely treated in the literature by experimental research works, analytical formulations and numerical implementations, with the objectives of understanding the tup-material interaction [8, 9], predicting the extent of induced damage [10, 11], and estimating the residual properties of the structure [7, 12, 13]. In particular, many research efforts have been spent to model impact history. To this aim, quite simple closed-form solutions [14], easy to use and effective, but restricted to simple impact cases due to the underlying simplifying assumptions [10, 14, 15], have been often employed.

In the last decades, an alternative to the analytical formulations has been offered by the numerical methodologies based on Finite Element (FE) approach. Since the onset of damage in a composite does not usually lead to ultimate failure, the ability of FE in simulating an impact event is critically dependent on its capacity to represent the sequence of damage modes, the conditions for delamination propagation, as well as the stiffness and strength degradation associated with the various damage states. FE

IMPACT IMPACT

90 0 90

90 0 0 Matrix cracking (shear failure)

Matrix cracking (tension failure) Delamination

16

formulations including failure criteria, plasticity theory, fracture mechanics, and damage mechanics. The main drawback of the failure criteria approach [16], initially adopted for unidirectional composites and developed for the static regime, is related to the impossibility to locate the position of the crack and to predict the crack sizes.

Moreover, the progressive degradation of stiffness material properties cannot be taken into account. Plasticity approach can be appropriate for composites exhibiting ductile behavior (e.g. thermoplastic composites), in combination with the failure criteria approach for damage prediction [17]. For such materials, a generalized anisotropic model in large strains, based on the classical isotropic plasticity theory, was presented by Car et al. [18]. The fracture mechanics approach [19] is based on the comparison of the strain energy at a crack front of known size with critical values of strain energy release rate. Zerbst et al. [20] applied this approach to predict residual compression strength and delamination growth in composites, showing appreciable results. The main disadvantage of fracture mechanics analysis is that it requires the definition of a pre-existing crack region in the numerical model. The Continuum Damage Mechanics (CDM) approach, initially introduced by Kachanov [21] and Rabotnov [22], has grown considerably in the past twenty years. According to CDM, damage is considered as a deterioration process of the material, introduced as part of the material definition.

Using CDM concept, Matzenmiller et al. [23] developed a mathematical model for damage of composite materials, connecting the damage level to the degraded elastic properties of the material, in turn depending on the particular damage mechanism (fiber breakage, fiber microbuckling, matrix cracking, etc.). This approach has been implemented in many research works [24-27], demonstrating promising results in predicting the impact response and damage extent.

**2.4. Materials and experimental methods **

The GFRP panels considered in this work were obtained from prepreg layers made
of E‐glass plain‐weave fabric, 295 g/m^{2} in areal weight, and Cycom 7701 epoxy resin.

An overview of the mechanical properties of the ply material, drawn from the manufacturer’s technical data sheet, is given in Tab. I (values in parentheses).

Two laminates, having stacking sequence [(0,90)n/(+45,‐45)n]s, with n=1,2 as
depicted in Figure 2.6a and b, respectively, were obtained and press cured for 2 hours
*at 120°C temperature and 0.1 MPa pressure. The nominal thickness t was 0.96 mm and *
*1.92 mm for n=1 and n=2, respectively. *

*a) b) *

**Figure 2.6: Schematic representation of the GFRP stacking sequence with n=1, a) and ****n=2, b). **

From the laminates, square specimens 70 mm in side were cut, and subjected to
low‐velocity impact tests using a Ceast MK4 instrumented testing machine, equipped
with a DAS 4000 digital acquisition system. The samples were clamped on a steel plate
with a circular opening 50 mm in diameter, and struck at their center using a
hemispherical steel impactor, 16 mm in diameter and 3.6 kg in mass. Various energy
*levels U, in the range 0.4 to 20 J were adopted, appropriately setting the tup height. *

For each impact energy level, three experimental tests were performed.

*Thanks to the translucent appearance of GFRP, the projected damage area A** _{p}* of
selected impacted samples was highlighted by an intense light source located at their

*back side, photographed, and the A*

*extent was measured through an image analyzer.*

_{p}*Then, the specimens were immersed in a blue ink bath, until A** _{p}* was fully darkened;

after that, they were carefully deplied with the help of moderate heating, and the extent of the delaminated areas found in correspondence of each interface was computed as the average measures of upper and lower delaminated areas of each ply, Am; the total delaminated area, Ad, was computed as the sum of the delaminated surfaces in correspondence of each interface.

**2.5. Experimental results and discussion **

*Typical F-d curves recorded during the impact tests, obtained for the two panel *
thicknesses, are collected in Figure 2.7. At low displacement, the material behavior is
substantially elastic, and disturbed by dynamic oscillations, more marked for the
thicker panel. As discussed in previous works [28, 29], the curvature affecting the

18

thinner laminate during this step is due to membrane effects. Beyond a given load
*threshold, dependent on the target thickness, sudden load drops appear in the F-d *
curves, indicating damage beginning and propagation. Nevertheless, the general trend
of the contact force increases further up to the maximum load, where a dramatic load
*drop, suggesting major damage, is observed. After that, the F-d curves flatten out until *
the maximum displacement, corresponding to a zero velocity, is achieved. During
rebound, the elastic portion of the energy stored into the material is transferred back to
*the impactor, whereas another portion (represented by the area enclosed in the F-d *
curve) is irreversibly absorbed through material damage, heat, and vibrations.

**Figure 2.7: Effect of the laminate thickness, t, on the F-d curves. **

As previously specified, the different energy levels in the tests were obtained
by suitably setting the drop height of the impactor, i.e. using different impact
*velocities. In Figure 2.8, different F-d curves, deriving from impact tests performed at *
increasing energy levels, are superposed. Despite some obvious differences,
attributable to the experimental scatter, the superposition is good. This indicates that,
within the experimental conditions adopted in the present tests, the material response is
not sensitive to velocity, so that energy is the true parameter affecting its response. In
*Figure 2.9, the irreversibly absorbed energy U** _{d}*, measured as the area enclosed within

*the F-d curve, is plotted against U (full symbols). As also found by other researchers*

0 400 800 1200 1600 2000 2400 2800 3200 3600 4000

0 2 4 6 8 10

**Fo****rce**** (****N)**

**Displacement (mm)**
t=1.92mm, U=15.5J

t=0.96mm, U=6.0J

[29], the trend is sensibly linear, with a slightly higher rate characterizing the thinner laminate.

**Figure 2.8: Effect of the energy level, U, on the F-d curves. Laminate thickness t=0.96mm. **

**Figure 2.9: Absorbed energy, U****d****, vs impact energy, U. **

0 400 800 1200 1600 2000

0 2 4 6 8 10

**Fo****rce**** (****N)**

**Displacement (mm)**

U=1.55 J U=3.32 J U=6.00 J

0 5 10 15 20 25

0 5 10 15 20 25

**Ab****so****rbe****d ****Energy **** (****J)**

**Impact Energy (J)**
Experimental t=0.96mm

Numerical t=0.96mm Experimental t=1.92mm Numerical t=1.92mm